The material described by NaZrTaSi2SO12 crystallizes in the monoclinic Cc space group. Na(1) is bonded in a distorted hexagonal planar geometry to one O(10), one O(11), one O(12), one O(7), one O(8), and one O(9) atom. Zr(1) is bonded to one O(1), one O(2), one O(3), one O(7), one O(8), and one O(9) atom to form ZrO6 octahedra that share corners with two equivalent Si(1)O4 tetrahedra, corners with two equivalent Si(2)O4 tetrahedra, and corners with two equivalent S(1)O4 tetrahedra. Ta(1) is bonded to one O(10), one O(11), one O(12), one O(4), one O(5), and one O(6) atom to form TaO6 octahedra that share corners with two equivalent Si(1)O4 tetrahedra, corners with two equivalent Si(2)O4 tetrahedra, and corners with two equivalent S(1)O4 tetrahedra. There are two inequivalent Si sites. In the first Si site, Si(1) is bonded to one O(1), one O(10), one O(4), and one O(7) atom to form SiO4 tetrahedra that share corners with two equivalent Zr(1)O6 octahedra and corners with two equivalent Ta(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 20-39°. In the second Si site, Si(2) is bonded to one O(11), one O(2), one O(6), and one O(9) atom to form SiO4 tetrahedra that share corners with two equivalent Zr(1)O6 octahedra and corners with two equivalent Ta(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 20-35°. S(1) is bonded to one O(12), one O(3), one O(5), and one O(8) atom to form SO4 tetrahedra that share corners with two equivalent Zr(1)O6 octahedra and corners with two equivalent Ta(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 26-35°. There are twelve inequivalent O sites. In the first O site, O(6) is bonded in a bent 150 degrees geometry to one Ta(1) and one Si(2) atom. In the second O site, O(7) is bonded in a 3-coordinate geometry to one Na(1), one Zr(1), and one Si(1) atom. In the third O site, O(8) is bonded in a 3-coordinate geometry to one Na(1), one Zr(1), and one S(1) atom. In the fourth O site, O(9) is bonded in a 3-coordinate geometry to one Na(1), one Zr(1), and one Si(2) atom. In the fifth O site, O(10) is bonded in a 3-coordinate geometry to one Na(1), one Ta(1), and one Si(1) atom. In the sixth O site, O(11) is bonded in a 3-coordinate geometry to one Na(1), one Ta(1), and one Si(2) atom. In the seventh O site, O(12) is bonded in a 3-coordinate geometry to one Na(1), one Ta(1), and one S(1) atom. In the eighth O site, O(1) is bonded in a bent 150 degrees geometry to one Zr(1) and one Si(1) atom. In the ninth O site, O(2) is bonded in a bent 150 degrees geometry to one Zr(1) and one Si(2) atom. In the tenth O site, O(3) is bonded in a bent 150 degrees geometry to one Zr(1) and one S(1) atom. In the eleventh O site, O(4) is bonded in a bent 150 degrees geometry to one Ta(1) and one Si(1) atom. In the twelfth O site, O(5) is bonded in a bent 150 degrees geometry to one Ta(1) and one S(1) atom. is represented by the Crystallographic Information File (CIF) [CIF]
data_NaZrTaSi2SO12
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   8.941
_cell_length_b   8.941
_cell_length_c   9.274
_cell_angle_alpha   90.236
_cell_angle_beta   118.639
_cell_angle_gamma   119.907
_symmetry_Int_Tables_number   1
_cell_volume   534.430
_cell_formula_units_Z   2
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Na  Na0  1  0.024  0.510  0.506  1.0
  Na  Na1  1  0.996  0.982  0.006  1.0
  O  O2  1  0.592  0.871  0.082  1.0
  O  O3  1  0.207  0.703  0.079  1.0
  O  O4  1  0.375  0.489  0.094  1.0
  O  O5  1  0.606  0.219  0.594  1.0
  O  O6  1  0.376  0.372  0.579  1.0
  O  O7  1  0.211  0.990  0.582  1.0
  O  O8  1  0.422  0.143  0.921  1.0
  O  O9  1  0.783  0.273  0.909  1.0
  O  O10  1  0.644  0.501  0.921  1.0
  O  O11  1  0.420  0.777  0.421  1.0
  O  O12  1  0.636  0.627  0.409  1.0
  O  O13  1  0.778  0.999  0.421  1.0
  O  O14  1  0.183  0.773  0.763  1.0
  O  O15  1  0.976  0.399  0.773  1.0
  O  O16  1  0.340  0.558  0.766  1.0
  O  O17  1  0.209  0.926  0.266  1.0
  O  O18  1  0.374  0.297  0.273  1.0
  O  O19  1  0.989  0.080  0.263  1.0
  O  O20  1  0.783  0.226  0.226  1.0
  O  O21  1  0.999  0.566  0.224  1.0
  O  O22  1  0.658  0.450  0.236  1.0
  O  O23  1  0.786  0.078  0.736  1.0
  O  O24  1  0.659  0.726  0.724  1.0
  O  O25  1  0.999  0.943  0.726  1.0
  S  S26  1  0.504  0.465  0.251  1.0
  S  S27  1  0.785  0.246  0.751  1.0
  Si  Si28  1  0.787  0.046  0.252  1.0
  Si  Si29  1  0.209  0.746  0.248  1.0
  Si  Si30  1  0.501  0.539  0.748  1.0
  Si  Si31  1  0.205  0.964  0.752  1.0
  Ta  Ta32  1  0.707  0.359  0.065  1.0
  Ta  Ta33  1  0.705  0.858  0.565  1.0
  Zr  Zr34  1  0.302  0.665  0.934  1.0
  Zr  Zr35  1  0.269  0.133  0.434  1.0
[/CIF]
.
The material described by NaZrTaSi2SO12 crystallizes in the monoclinic Cc space group. Na(1) is bonded in a distorted hexagonal planar geometry to one O(10), one O(11), one O(12), one O(7), one O(8), and one O(9) atom. Zr(1) is bonded to one O(1), one O(2), one O(3), one O(7), one O(8), and one O(9) atom to form ZrO6 octahedra that share corners with two equivalent Si(1)O4 tetrahedra, corners with two equivalent Si(2)O4 tetrahedra, and corners with two equivalent S(1)O4 tetrahedra. Ta(1) is bonded to one O(10), one O(11), one O(12), one O(4), one O(5), and one O(6) atom to form TaO6 octahedra that share corners with two equivalent Si(1)O4 tetrahedra, corners with two equivalent Si(2)O4 tetrahedra, and corners with two equivalent S(1)O4 tetrahedra. There are two inequivalent Si sites. In the first Si site, Si(1) is bonded to one O(1), one O(10), one O(4), and one O(7) atom to form SiO4 tetrahedra that share corners with two equivalent Zr(1)O6 octahedra and corners with two equivalent Ta(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 20-39°. In the second Si site, Si(2) is bonded to one O(11), one O(2), one O(6), and one O(9) atom to form SiO4 tetrahedra that share corners with two equivalent Zr(1)O6 octahedra and corners with two equivalent Ta(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 20-35°. S(1) is bonded to one O(12), one O(3), one O(5), and one O(8) atom to form SO4 tetrahedra that share corners with two equivalent Zr(1)O6 octahedra and corners with two equivalent Ta(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 26-35°. There are twelve inequivalent O sites. In the first O site, O(6) is bonded in a bent 150 degrees geometry to one Ta(1) and one Si(2) atom. In the second O site, O(7) is bonded in a 3-coordinate geometry to one Na(1), one Zr(1), and one Si(1) atom. In the third O site, O(8) is bonded in a 3-coordinate geometry to one Na(1), one Zr(1), and one S(1) atom. In the fourth O site, O(9) is bonded in a 3-coordinate geometry to one Na(1), one Zr(1), and one Si(2) atom. In the fifth O site, O(10) is bonded in a 3-coordinate geometry to one Na(1), one Ta(1), and one Si(1) atom. In the sixth O site, O(11) is bonded in a 3-coordinate geometry to one Na(1), one Ta(1), and one Si(2) atom. In the seventh O site, O(12) is bonded in a 3-coordinate geometry to one Na(1), one Ta(1), and one S(1) atom. In the eighth O site, O(1) is bonded in a bent 150 degrees geometry to one Zr(1) and one Si(1) atom. In the ninth O site, O(2) is bonded in a bent 150 degrees geometry to one Zr(1) and one Si(2) atom. In the tenth O site, O(3) is bonded in a bent 150 degrees geometry to one Zr(1) and one S(1) atom. In the eleventh O site, O(4) is bonded in a bent 150 degrees geometry to one Ta(1) and one Si(1) atom. In the twelfth O site, O(5) is bonded in a bent 150 degrees geometry to one Ta(1) and one S(1) atom. is represented by the Crystallographic Information File (CIF) [CIF]
data_NaZrTaSi2SO12
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   8.941
_cell_length_b   8.941
_cell_length_c   9.274
_cell_angle_alpha   90.236
_cell_angle_beta   118.639
_cell_angle_gamma   119.907
_symmetry_Int_Tables_number   1
_cell_volume   534.430
_cell_formula_units_Z   2
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Na  Na0  1  0.024  0.510  0.506  1.0
  Na  Na1  1  0.996  0.982  0.006  1.0
  O  O2  1  0.592  0.871  0.082  1.0
  O  O3  1  0.207  0.703  0.079  1.0
  O  O4  1  0.375  0.489  0.094  1.0
  O  O5  1  0.606  0.219  0.594  1.0
  O  O6  1  0.376  0.372  0.579  1.0
  O  O7  1  0.211  0.990  0.582  1.0
  O  O8  1  0.422  0.143  0.921  1.0
  O  O9  1  0.783  0.273  0.909  1.0
  O  O10  1  0.644  0.501  0.921  1.0
  O  O11  1  0.420  0.777  0.421  1.0
  O  O12  1  0.636  0.627  0.409  1.0
  O  O13  1  0.778  0.999  0.421  1.0
  O  O14  1  0.183  0.773  0.763  1.0
  O  O15  1  0.976  0.399  0.773  1.0
  O  O16  1  0.340  0.558  0.766  1.0
  O  O17  1  0.209  0.926  0.266  1.0
  O  O18  1  0.374  0.297  0.273  1.0
  O  O19  1  0.989  0.080  0.263  1.0
  O  O20  1  0.783  0.226  0.226  1.0
  O  O21  1  0.999  0.566  0.224  1.0
  O  O22  1  0.658  0.450  0.236  1.0
  O  O23  1  0.786  0.078  0.736  1.0
  O  O24  1  0.659  0.726  0.724  1.0
  O  O25  1  0.999  0.943  0.726  1.0
  S  S26  1  0.504  0.465  0.251  1.0
  S  S27  1  0.785  0.246  0.751  1.0
  Si  Si28  1  0.787  0.046  0.252  1.0
  Si  Si29  1  0.209  0.746  0.248  1.0
  Si  Si30  1  0.501  0.539  0.748  1.0
  Si  Si31  1  0.205  0.964  0.752  1.0
  Ta  Ta32  1  0.707  0.359  0.065  1.0
  Ta  Ta33  1  0.705  0.858  0.565  1.0
  Zr  Zr34  1  0.302  0.665  0.934  1.0
  Zr  Zr35  1  0.269  0.133  0.434  1.0
[/CIF]
.